advertisement

1 1.1 X-ray-reflectometry (XRR) Motivation Most technological applications of thin films require films of definite thickness. This is because most properties of thin films are thickness dependent. Hence, determination of film thickness with high precision is very crucial for these technologies. XRR is a non-destructive and non-contact technique for thickness determination between 2-200 nm with a precision of about 1-3 Å. In addition to thickness determination, this technique is also employed for the determination of density and roughness of films and also multilayers with a high precision. 1.2 The Principle XRR method involves monitoring the intensity of the x-ray beam reflected by a sample at grazing angles. A monochromatic x-ray beam of wavelength λ irradiates a sample at a grazing angle ω and the reflected intensity at an angle 2θ is recorded Figure 1: θ/2θ-Scan: The condition of incident angle ω = (2θ)/2 = θ = outgoing angle is satisfied. The detector D rotates at twice the speed of the sample P. This arrangement is sensitive only to the planes parallel to the surface of the sample. The beam makes an incident angle ω with the surface of the sample P. The reflected intensity at angle of 2θ is measured. Both the rotation of the sample ω and the detector (2θ) are about the same axis MP (perpendicular to the drawing). The sample is adjusted so that the rotation axis lies on the sample surface. The Detector circle is fixed through the (programmable) detector slit(PRS, programmable receiving slit). The anode focus, F of the tube lies on the detector circle. 1 by a detector, see figure 1. This figure illustrates specular reflection where the condition ω = 2θ/2 is satisfied. The mode of operation is therefore θ/2θ mode which make sure the incident angle is always half of the angle of diffraction. The reflection at the surface and interfaces is due to the different electron densities in the different layers (films), which corresponds to different reflective indexes in the classical optics. For incident angles θ below a critical angle θc , total external reflection occurs. The critical angle for most materials is less than 0.3◦ . The density of the material is determined from the critical angle. Above θc the reflection from the different interfaces interfere and give rise to interference fringes. The period of the interference fringes and the fall in the intensity are related to the thickness and the roughness of the layer (layers in case of multilayers). The reflection can be analyzed using the classical theory (Fresnel equation). The typical range for these measurements are between 0◦ and 5◦ in θ. 1.2.1 Film density The complex refractive index in the x-ray region is slightly less than 1 and is given by ñ = 1 − δ + iβ (1) where δ and β represent the dispersion and absorption, respectively. For frequencies far greater than the resonance frequencies, ϑ0 , of the atom δ can be given by the expression e2 ne r0 λ2 2 δ= λ = · ne (2) 2ε0 m(2πc)2 2π where r0 is the Bohr atomic radius and ne is the electron density. The electron density is given by ne = Z · nAtom where Z is the number of electrons per atom. For a more precise expression of δ, Z is usually replaced with the a complex atom form factor f˜ = f0 + f 0 + if 00 = Z + f 0 + if 00 . The term f 0 + if 00 is due to dispersion and absorption and describes the x-ray absorption edge. It follows that r0 λ2 · (Z + f 0 ) · nAtom 2π r0 λ2 00 β = · f · nAtom . 2π δ = and (3) (4) The magnitudes of δ and β are of the order of 10−5 and 10−6 , respectively. Since the atomic concentration is given as nAtom = NA ·ρ A it is apparent that, the density of the material can be determined from the values of δ and β. Here NA is the Avogadros number and A the atomic weight. The 2 Figure 2: XRR-measurements and simulations of an Tungsten oxide film on glass. The films were deposited using different deposition parameters. A shift in the total reflection edge is apparent which implies a change in density. The sample with the lowest density (lowest reflection edge) exhibits interference fringes in a shorter angular range than the sample with higher density. This implies that the roughness of the sample with lower density is higher than the roughness of the sample with higher density. The thickness of the samples are obtained from the period of the oscillations. density of a compound material of known stoichiometry can also be determined from δ and β with slight modifications in the formula. We illustrate the determination of the different quantities obtained from XRR measurement with an example of a single film on a substrate. For qualitative discussion, it is adequate to consider an absorption free film i.e β = 0 but it should be noted that β cannot be ignored in the simulation of XRR measurements. We consider reflection at an interface between air, nair = 1 and another material, n1 = 1 − δ. For incident angles below a critical angle, θc , (θ < θc ), total reflection occurs. By applying Snell’s law and small angle approximations, the critical angle, θc can be expressed as 1 − δ = cos θC θ2 ≈ 1− C √ 2 ⇔ θC ≈ 2δ r r0 λ2 (Z + f 0 ) = NA ·ρ π A A typical measurement is shown in fig. 2 where the total reflection angle is determined by the abrupt fall in the reflected intensity. 3 1.2.2 Film thickness For incident angles greater than θc , (θ > θc ) the x-ray beam penetrates inside the film. Reflection therefore occurs at the top and the bottom surfaces of the film. The interference between the rays reflected from the top and the bottom of the film surfaces results in interference fringes which does not depend on the frequency like in the case of optical spectroscopy but are angle dependent. Due to the low amplitude reflection coefficient (ρv,h ∼ 1/ sin2 θ ⇒ Rv,h = |rv,h | ∼ 1/ sin4 θ ≈ 1/θ4 ) of interface between adjacent layers, contributions of multiply reflected beams can be neglected. The m-th interference maximum for a path difference ∆ = mλ,is located at mλ = ∆ = 2dÑX,1 (θm ) p 2 − 2δ ≈ 2d θm λ2 2 ⇔ θm ≈ m2 2 + 2δ 4d λ2 = m2 2 + θC2 . 4d (5) mit m ∈ N. (6) (7) (8) If the substrate is optically denser than the film, a phase difference of π occurs at the reflection film / substrate interface and m is substituted with m+ 12 . Employing equation (7) and the difference between two neighboring maxima and minima, the thickness can be determined and is given by λ 1 p p 2 2 2 − θ2 2 θm+1 − θC − θm C 1 λ , f”ur θm θC . ≈ 2 θm+1 − θm d ≈ (9) (10) The thickness is often determined with a precision better than 1 Å for measurements exhibiting interference fringes in a bigger angular range. The thickness influence is illustrated in fig. 2. 1.2.3 Surface Roughness Another important quantity determined from XRR measurements is the surfaceand interface-roughness. Roughness gives rise to diffuse scattering, resulting to a less intensity in the specularly reflected beam. General scattering formalism have been developed that calculate the scattered fields for both specular and nonspecular scattering. In one of the formalism, Névot and Croce considered roughness by assuming non-homogeneous thickness. They assumed that the thickness has a gaussian distribution with a mean d and a standard deviation σ. With this 4 assumption, they corrected the Fresnel coefficients of reflection ρv,h as d ρv,h · exp − 2 2σ The influence of roughness is clearly shown in the fig. 2 1.3 Example The switching kinetics of Tungsten oxide (see optical active films) due to hydrogen presence mainly depend on the porosity of the films. The switching processes for highly porous films are faster than for films with low porosity. By varying the deposition parameters, films of different porosity are sputtered using a locally assembled sputtering unit. XRR technique is used to determine the development of density and roughness of the films and these results are compared with the results of the switching kinetics. An XRR measurement is shown in fig. 2. 5